fabrication and optimization of nanodiamonds-composited ... fabrication and optimization of...
Click here to load reader
Post on 29-Jan-2021
Embed Size (px)
RESEARCH ARTICLE Open Access
Fabrication and optimization of Nanodiamonds-composited poly(ε- caprolactone) fibrous matrices for potential regeneration of hard tissues Guk Young Ahn†, Tae-Kyung Ryu†, Yu Ri Choi, Ju Ri Park, Min Jeong Lee and Sung-Wook Choi*
Background: Electrospun fibrous matrices are of great importance for tissue engineering and drug delivery device. However, relatively low mechanical strength of the fibrous matrix is one of the major disadvantages. NDs with a positive charge were selected to enhance the mechanical property of a composited fibrous matrix by inducing the intermolecular interaction between NDs and polymer chain. We prepared ND-composited poly (ε-caprolactone) (PCL) fibrous matrices by electrospinning and evaluated their performance in terms of mechanical strength and cell behaviors.
Methods: A predetermined amounts of NDs (0.5, 1, 2 and 3 wt%) were added into PCL solution in a mixture of chloroform and 2,2,2-trifluoroethanol (8:2). ND-composited PCL (ND/PCL) fibrous matrices were prepared by electrospinning method. The tensile properties of the ND/PCL fibrous matrices were analyzed by using a universal testing machine. Mouse calvaria-derived preosteoblast (MC3T3-E1) was used for cell proliferation, alkaline phosphatase (ALP) assay, and Alizarin Red S staining.
Results: The diameters of the fibrous matrices were adjusted to approximately 1.8 μm by changing process variables. The intermolecular interaction between NDs and PCL polymers resulted in the increased tensile strength and the favorable interfacial adhesion in the ND/PCL fibrous matrices. The ND/PCL fibrous matrix with 1 wt% of ND had the highest tensile strength among the samples and also improved proliferation and differentiation of MC3T3- E1 cells.
Conclusions: Compared to the other samples, the ND/PCL fibrous matrix with 1 wt% of ND concentration exhibited superior performances for MC3T3 cells. The ND/PCL fibrous matrix can be potentially used for bone and dental tissue engineering.
Keywords: Biodegradable polymer, Composite, Nanodiamond, Electrospinning, Guided tissue engineering
Background Electrospun fibrous matrices are very useful in tissue engineering because of their large surface area, high aspect ratio, porosity, and the presence of very small pore structures on the fibers [1–3]. Most importantly, the topological structure of the electrospun products can mimic the extracellular matrix and enhance both
cell migration and proliferation . Many researchers have demonstrated the production of fibrous structures from various organic/inorganic materials and also prepared organic/inorganic composite fibers [5, 6]. Fur- thermore, several groups have investigated composite fibers with a therapeutic agent and functional materials using the electrospinning method. Zhang et al. fabricated electrospun biomimetic composited chitosan nanofibers containing hydroxyapatite (HAp) and confirmed the bone forming ability as shown by the cell proliferation, mineral deposition and morphology
* Correspondence: firstname.lastname@example.org †Guk Young Ahn and Tae-Kyung Ryu contributed equally to this work. Department of Biotechnology, The Catholic University of Korea, 43 Jibong-ro, Wonmi-gu, Bucheon-si, Gyeonggi-do 420-743, Republic of Korea
© The Author(s). 2018 Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The Creative Commons Public Domain Dedication waiver (http://creativecommons.org/publicdomain/zero/1.0/) applies to the data made available in this article, unless otherwise stated.
Ahn et al. Biomaterials Research (2018) 22:16 https://doi.org/10.1186/s40824-018-0126-x
http://crossmark.crossref.org/dialog/?doi=10.1186/s40824-018-0126-x&domain=pdf mailto:email@example.com http://creativecommons.org/licenses/by/4.0/ http://creativecommons.org/publicdomain/zero/1.0/
observation . Li et al. designed and evaluated the Silk fibroin fibrous scaffolds containing bone morphogenetic protein-2 and HAp nanopowders for bone tissue engineering . Ma et al. reported enzymatic degradable hydrogels based on collagen and alendronate conjugated HAp nanoparticles. These hydrogels demonstrated ex- cellent biocompatibility and promoted the adhesion and proliferation of MC3T3-E1 cells . Yang et al. were successful in coating electrospun poly(ε-caprolactone) (PCL) with a thin layer of calcium phosphate for bone tissue engineering . Rajzer et al. prepared an electro- spun bi-layer fibrous scaffold using PCL and gelatin modified with calcium phosphate for bone mineralization . Cao et al. fabricated beta-tricalcium phosphate (β-TCP) composited poly(glycolic acid) three-dimensional scaffolds using solvent casting and particle leaching method and evaluated their biocompatibility, osteocon- ductivity, osteogenesis and degradation in vivo . In general, the materials for the enhancement of osteocon- duction have been limited to inorganics such as HAp and calcium phosphates. Carbon-based materials, including fullerene, graphene,
carbon nanotubes, graphite, nanohorns and nanodia- monds (NDs), have also been investigated for various biomedical applications [13, 14]. Depan et al. investi- gated the biological response of graphene conjugated chitosan scaffolds and reported their higher mechanical properties, lower degradation rate, and enhanced osteo- blast cell growth . Pan et al. prepared the multiwall carbon nanotubes/PCL composite scaffolds using solu- tion evaporation technique and evaluated the prolifera- tion and differentiation of bone marrow stromal cells . Recently, NDs, which are carbon-based allotrope nanoparticles of truncated octahedral composition, have attracted attention as an innovative nanomaterial be- cause of their high biocompatibility, spherical morph- ology, high density, surface functionality, and strong hardness . Many researchers have reported on the excellent non-toxicity and biocompatibility of NDs using a variety of cells such as epithelial cell, adenocarcinoma cell, neuroblastoma cell, and so on [18, 19]. Grausova et al. designed silicon films with NDs and confirmed the enhanced adhesion, spreading, viability, growth, and maturation of human osteoblast-like MG63 cells on these films . Zhang et al. fabricated fluorescent poly(L-lactic acid)-ND composite thin film and demon- strated the enhanced proliferation and differentiation of osteoblasts on this film as well as an increased mechan- ical strength of the scaffold . In view of these inter- esting applications, a systematic study of the effect of NDs used as composite materials for tissue engineering is crucial. Recently, our group prepared bone-targeted drug
carriers conjugated with NDs and found that NDs itself
increased the alkaline phosphatase (ALP) activity . By inspiring our previous results, NDs with a positive charge were composited in a fibrous matrix in an effort to enhance the mechanical strength and cellular behaviors on the fibrous matrix. We fabricated ND-composited PCL (ND/PCL) matrices using the elec- trospinning method for guided tissue engineering and optimized the ND concentrations in terms of the tensile properties of the matrix and the proliferation and differ- entiation of preosteoblast. We believe that the PCL/ND matrices have great potential applications for regener- ation of hard tissues.
Methods Preparation of ND/PCL fibrous matrices Fibrous matrices were produced using a horizontal electrospinning setup . Polycaprolactone (PCL, Mw = 80,000, Sigma–Aldrich), chloroform (CF, Sigma– Aldrich), and 2,2,2-trifluoroethanol (TFE, Sigma-Aldrich) were used to fabricate the ND/PCL fibrous matrices. NDs with a positive charge (46.0 ± 3.4 mV) were purchased from Neomond Ltd. (Bucheon, Korea). The NDs were an- alyzed using the Zetasizer (Malvern Instruments Ltd., Worcestershire, UK) to determine their zeta potentials. For the preparation of the PCL fibrous matrix, PCL solu- tion (10 mL, 10 wt%, dissolved in CF:TFE = 8:2) was elec- trospun onto the aluminum dish using a syringe pump (NE-1000, New Era Pump Systems Inc., New York, USA). A high voltage was applied between the spinneret (a 24 G needle) and the collector located 15 cm away . The syringe was horizontally fixed on the syringe pump and the PCL and ND/PCL solutions were electrospun onto an aluminum foil collector. The ND concentration of the ND/PCL solution was varied as 0.5, 1, 2, and 3 wt%. In order to ensure that their diameter were similar, the fibers were fabricated under different conditions of applied voltage and flow rate .
Characterization of the ND/PCL fibrous matrix Scanning electron microscopy (SEM, S-4800, Hitachi High-Technologies, Co. Ltd., Tokyo, Japan) was used to characterize the morphologies of the ND/PCL fibrous matrices. The diameters of the fibers were calculated from the SEM images of the samples by analyzing at least 300 fibers using the ImageJ® software (National In- stitutes of Health, Bethesda, USA). The tensile properties of the ND/PCL fibrous matrices were analyzed by using a universal testing machine (UTM, LR 10 K, Lloyd in- struments Ltd., London, UK). The dimensions of the fi- brous matrices were 10 mm × 80 mm × 1 mm (width × length × thickness). The thickness of the fibrous matrix was measured with digital caliper. The extension rate was maintained at 5 mm/min at room temperature. The load cell was 50 N with a gauge length of 50 mm.
Ahn et al. Biomaterials